Pyroelectricity(Redirected from Pyroelectric)
Pyroelectricity (from the Greek pyr, fire, and electricity) is the property of certain crystals which are naturally electrically polarized and as a result contain large electric fields. The most important example is the gallium nitride semiconductor. The large electric fields in this material are unwanted for light emitting diodes (LEDs), but are very helpful for the fabrication of power transistors. Alternatively, pyroelectricity is interpreted as the ability of certain materials to generate a temporary voltage when they are heated or cooled. The change in temperature modifies the positions of the atoms slightly within the crystal structure, such that the polarization of the material changes. This polarization change gives rise to a voltage across the crystal. If the temperature stays constant at its new value, the pyroelectric voltage gradually disappears due to leakage current (the leakage can be due to electrons moving through the crystal, ions moving through the air, current leaking through a voltmeter attached across the crystal, etc.).
Pyroelectricity should not be confused with thermoelectricity, a different thermal effect with a different mechanism.
Pyroelectricity can be visualized as one side of a triangle, where each corner represents energy states in the crystal: kinetic, electrical and thermal energy. The side between electrical and thermal corners represents the pyroelectric effect and produces no kinetic energy. The side between kinetic and electrical corners represents the piezoelectric effect and produces no heat.
Pyroelectric charge in minerals develops on the opposite faces of asymmetric crystals. The direction in which the propagation of the charge tends toward is usually constant throughout a pyroelectric material, but, in some materials, this direction can be changed by a nearby electric field. These materials are said to exhibit ferroelectricity. All pyroelectric materials are also piezoelectric, the two properties being closely related. However, note that some piezoelectric materials have a crystal symmetry that does not allow pyroelectricity.
The property of pyroelectricity is the measured change in net polarization (a vector) proportional to a change in temperature. The total pyroelectric coefficient measured at constant stress is the sum of the pyroelectric coefficients at constant strain (primary pyroelectric effect) and the piezoelectric contribution from thermal expansion (secondary pyroelectric effect). Under normal circumstances, even polar materials do not display a net dipole moment. As a consequence there are no electric dipole equivalents of bar magnets because the intrinsic dipole moment is neutralized by "free" electric charge that builds up on the surface by internal conduction or from the ambient atmosphere. Polar crystals only reveal their nature when perturbed in some fashion that momentarily upsets the balance with the compensating surface charge.
Spontaneous polarization is temperature dependent, so a good perturbation probe is a change in temperature which induces a flow of charge to and from the surfaces. This is the pyroelectric effect. All polar crystals are pyroelectric, so the 10 polar crystal classes are sometimes referred to as the pyroelectric classes. The property of pyroelectric crystal is to measure change in net polarization (a vector) proportional to a change in temperature. The total pyroelectric coefficient measured at constant stress is the sum of the pyroelectric coefficients at constant strain (primary pyroelectric effect) and the piezoelectric contribution from thermal expansion (secondary pyroelectric effect). Pyroelectric materials can be used as infrared and millimeter wavelength detectors.
Electret is the electrical equivalent of a permanent magnet.
The pyroelectric coefficient may be described as the change in the spontaneous polarization vector with temperature:
where pi (Cm−2K−1) is the vector for the pyroelectric coefficient.
The first reference to the pyroelectric effect is in writings by Theophrastus in 314 BC, who noted that lyngourion, tourmaline, could attract sawdust or bits of straw when heated. Tourmaline's properties were rediscovered in 1707 by Johann Georg Schmidt, who noted that the stone attracted only hot ashes, not cold ones. In 1717 Louis Lemery noticed, as Schmidt had, that small scraps of non-conducting material were first attracted to tourmaline, but then repelled by it once they contacted the stone. In 1747 Linnaeus first related the phenomenon to electricity (he called tourmaline Lapidem Electricum, "the electric stone"), although this was not proven until 1756 by Franz Ulrich Theodor Aepinus.
Research in pyroelectricity became more sophisticated in the 19th century. In 1824 Sir David Brewster gave the effect the name it has today. Both William Thomson in 1878 and Woldemar Voigt in 1897 helped develop a theory for the processes behind pyroelectricity. Pierre Curie and his brother, Jacques Curie, studied pyroelectricity in the 1880s, leading to their discovery of some of the mechanisms behind piezoelectricity.
All crystal structures can be divided into 32 crystal classes, according to the number of rotational axes and reflection planes they exhibit that leave the crystal structure unchanged. Of the thirty-two crystal classes, twenty-one are non-centrosymmetric (not having a centre of symmetry). Of these twenty-one, twenty exhibit direct piezoelectricity, the remaining one being the cubic class 432. Ten of these twenty piezoelectric classes are polar, i.e., they possess a spontaneous polarization, having a dipole in their unit cell, and exhibit pyroelectricity. If this dipole can be reversed by the application of an electric field, the material is said to be ferroelectric. Any dielectric material develops a dielectric polarization (electrostatics) when an electric field is applied, but a substance which has such a natural charge separation even in the absence of a field is called a polar material. Whether or not a material is polar is determined solely by its crystal structure. Only 10 of the 32 point groups are polar. All polar crystals are pyroelectric, so the ten polar crystal classes are sometimes referred to as the pyroelectric classes.
Piezoelectric crystal classes: 1, 2, m, 222, mm2, 4, -4, 422, 4mm, -42m, 3, 32, 3m, 6, -6, 622, 6mm, -62m, 23, -43m
Pyroelectric: 1, 2, m, mm2, 3, 3m, 4, 4mm, 6, 6mm
Two effects which are closely related to pyroelectricity are ferroelectricity and piezoelectricity. Normally materials are very nearly electrically neutral on the macroscopic level. However, the positive and negative charges which make up the material are not necessarily distributed in a symmetric manner. If the sum of charge times distance for all elements of the basic cell does not equal zero the cell will have an electric dipole moment which is a vector quantity. The dipole moment per unit volume is defined as the dielectric polarization. If this dipole moment changes with the effect of applied temperature changes, applied electric field, or applied pressure, the material is pyroelectric, ferroelectric, or piezoelectric, respectively.
The ferroelectric effect is exhibited by materials which possess an electric polarization in the absence of an externally applied electric field such that the polarization can be reversed if the electric field is reversed. Since all ferroelectric materials exhibit a spontaneous polarization, all ferroelectric materials are also pyroelectric (but not all pyroelectric materials are ferroelectric).
The piezoelectric effect is exhibited by crystals (such as quartz or ceramic) for which an electric voltage across the material appears when pressure is applied. Similar to pyroelectric effect, the phenomenon is due to the asymmetric structure of the crystals that allows ions to move more easily along one axis than the others. As pressure is applied, each side of the crystal takes on an opposite charge, resulting in a voltage drop across the crystal.
Pyroelectricity should not be confused with thermoelectricity: In a typical demonstration of pyroelectricity, the whole crystal is changed from one temperature to another, and the result is a temporary voltage across the crystal. In a typical demonstration of thermoelectricity, one part of the device is kept at one temperature and the other part at a different temperature, and the result is a permanent voltage across the device as long as there is a temperature difference. Both effects convert temperature change to electrical potential, but the pyroelectric effect converts temperature change over time into electrical potential, while the thermoelectric effect converts temperature change with position into electrical potential.
Progress has been made in creating artificial pyroelectric materials, usually in the form of a thin film, out of gallium nitride (GaN), caesium nitrate (CsNO3), polyvinyl fluorides, derivatives of phenylpyridine, and cobalt phthalocyanine. Lithium tantalate (LiTaO3) is a crystal exhibiting both piezoelectric and pyroelectric properties, which has been used to create small-scale nuclear fusion ("pyroelectric fusion").
Very small changes in temperature can produce an electric potential, due to a materials' pyroelectricity. Passive infrared sensors are often designed around pyroelectric materials, as the heat of a human or animal from several feet away is enough to generate a difference in charge.
A pyroelectric can be repeatedly heated and cooled (analogously to a heat engine) to generate usable electrical power. One group calculated that a pyroelectric in an Ericsson cycle could reach 50% of Carnot efficiency, while a different study found a material that could, in theory, reach 84-92% of Carnot efficiency (these efficiency values are for the pyroelectric itself, ignoring losses from heating and cooling the substrate, other heat-transfer losses, and all other losses elsewhere in the system). Possible advantages of pyroelectric generators for generating electricity (as compared to the conventional heat engine plus electrical generator) include: potentially lower operating temperatures, less bulky equipment, and fewer moving parts. Although a few patents have been filed for such a device, it does not appear to be anywhere close to commercialization yet.
- Ashcroft, N. W. & Mermin, N. D. Solid State Physics. (Cengage Learning, 1976).
- Gallium Nitride (GaN): Physics, Devices, and Technology.” 2015. CRC Press. October 16
- Charles Kittel-8th Edition. 2016. Introduction to Solid State Physics.
- Webster, John G (1999). The measurement, instrumentation, and sensors handbook. pp. 32–113. ISBN 978-0-8493-8347-2.
- In this article, the term "voltage" is used in the everyday sense, i.e. what a voltmeter measures. This is actually the electrochemical potential, not the electrostatic potential (Galvani potential).
- Buchanan, Relva C. (2004). Ceramic Materials for Electronics: Third Edition, Revised and Expanded (Third ed.). Cincinnati, Ohio: Marcel Dekker, Inc. p. 217. ISBN 0-8247-4028-9. Retrieved 10 November 2015.
- Damjanovic, Dragan, 1998, Ferroelectric, dielectric and piezoelectric properties of ferroelectric thin films and ceramics, Rep. Prog. Phys. 61, 1267–1324.
- Earle R. Caley and John F.C. Richards, Theophrastus: On Stones (Columbus, Ohio: Ohio State University, 1956), page 51, paragraph 28 of the original text: "It [smaragdos] is remarkable in its powers, and so is the lyngourion [i.e., lynx-urine stone] … . It has the power of attraction, just as amber has, and some say that it not only attracts straws and bits of wood, but also copper and iron, if the pieces are thin, as Diokles used to explain."
- Johann Georg Schmidt, Curiöse Speculationes bey Schalflosen Nächten [Curious Speculations During Sleepless Nights] (Chemnitz and Leipzig (Germany): Conrad Stössen, 1707), pages 269-270. An English translation of the relevant passage appears in: Sidney B. Lang, Sourcebook of Pyroelectricity, vol. 2 (New York, New York: Gordon and Breach, 1974), page 96.
- "Diverse observations de la physique generale," Histoire de l'Académie des Sciences (1717); see pages 7-8.
- Carl von Linné ("Linnaeus"), Flora Zeylanica: Sistens Plantas Indicas Zeylonae Insulae [The Flora of Ceylon: consisting of Indian plants of the island of Ceylon] (Stockholm ("Holmiae"), Sweden: Laurentii Salvii, 1747), page 8. A translation of the relevant passage appears in Lang (1974), page 103.
- Aepinus (1756) "Memoire concernant quelques nouvelles experiences électriques remarquables" [Memoir concerning some remarkable new electrical experiments], Histoire de l'Académie royale des sciences et des belles lettres (Berlin), vol. 12, pages 105-121.
- Brewster, David (1824). "Observations of the pyro-electricity of minerals". The Edinburgh Journal of Science. 1: 208–215.
- William Thomson (1878) "On the thermoelastic, thermomagnetic and pyroelectric properties of matter," Philosophical Magazine, series 5, vol. 5, pages 4 - 26.
- W. Voigt (1897) "Versuch zur Bestimmung des wahren specifischen electrischen Momentes eines Turmalins" (Experiment to determine the true specific electric moment of a tourmaline), Annalen der Physik, vol. 60, pages 368 - 375.
- Naranjo, B.; Gimzewski, J.K.; Putterman, S. (2005). "Observation of nuclear fusion driven by a pyroelectric crystal". Nature. 434 (7037): 1115–1117. Bibcode:2005Natur.434.1115N. doi:10.1038/nature03575. ISSN 0028-0836. PMID 15858570.
- Sebald, Gael; Pruvost, Sebastien; Guyomar, Daniel (2008). "Energy harvesting based on Ericsson pyroelectric cycles in a relaxor ferroelectric ceramic" (PDF). Smart Materials and Structures. 17: 015012. Bibcode:2008SMaS...17a5012S. doi:10.1088/0964-1726/17/01/015012.
- Sebald, Gael; Guyomar, Daniel; Agbossou, Amen (2009). "On thermoelectric and pyroelectric energy harvesting". Smart Materials and Structures. 18: 125006. Bibcode:2009SMaS...18l5006S. doi:10.1088/0964-1726/18/12/125006.
- Olsen, Randall B.; Evans, Diane (1983). "Pyroelectric energy conversion: Hysteresis loss and temperature sensitivity of a ferroelectric material". Journal of Applied Physics. 54: 5941. Bibcode:1983JAP....54.5941O. doi:10.1063/1.331769.
- Kouchachvili, L; Ikura, M (2007). "Pyroelectric conversion—Effects of P(VDF–TrFE) preconditioning on power conversion". Journal of Electrostatics. 65: 182. doi:10.1016/j.elstat.2006.07.014.
- For example: US Patent 4647836, US Patent 6528898, US Patent 5644184
- Substantial explanations of pyroelectric detector operation
- Pyroelectric Infrared Detectors DIAS Infrared
- DoITPoMS Teaching and Learning Package- "Pyroelectric Materials"
- Lithium Tantalate (LiTaO3)
- Lithium Tantalate (LiTaO3)
- laser detection with lithium tantalate
- Strontium Barium Niobate (SrBaNb2O6)
- Strontium Barium Niobate (SrBaNb2O6)